 •Foreword
 •Foreword to First Edition
 •Contributors
 •Preface
 •A.1 Piezoelectric Materials
 •A.3 Optical Fiber Sensors
 •A.4 Electrorheological Fluids
 •A.5 Magnetostrictive Materials
 •A.6 MicroElectroMechanical Systems
 •A.7 Comparison Of Actuators
 •References
 •Index
 •1. Introduction and Overview
 •1.1 General
 •1.3 HighPerformance Fiber Composite Concepts
 •1.4 Fiber Reinforcements
 •1.5 Matrices
 •References
 •Bibliography
 •2. Basic Principles of Fiber Composite Materials
 •2.1 Introduction to Fiber Composite Systems
 •2.3 Micromechanics
 •2.4 Elastic Constants
 •2.5 Micromechanics Approach to Strength
 •2.6 Simple Estimate of Compressive Strength
 •References
 •3. Fibers for PolymerMatrix Composites
 •3.1 Overview
 •3.3 Carbon Fibers
 •3.4 Boron Fibers
 •3.5 Silicon Carbide
 •3.6 Aramid Fibers
 •3.7 Orientated Polyethylene Fibers
 •3.8 Dry Fiber Forms
 •References
 •4. Polymeric Matrix Materials
 •4.1 Introduction
 •4.2 Thermoset and Thermoplastic Polymer Matrix Materials
 •4.3 Thermosetting Resin Systems
 •4.4 Thermoplastic Systems
 •References
 •5. Component Form and Manufacture
 •5.1 Introduction
 •5.2 Outline of General Laminating Procedures
 •5.5 Filament Winding
 •5.7 Process Modelling
 •5.8 Tooling
 •References
 •6. Structural Analysis
 •6.1 Overview
 •6.2 Laminate Theory
 •6.3 Stress Concentration and Edge Effects
 •6.4 Failure Theories
 •6.7 Buckling
 •6.8 Summary
 •References
 •7. Mechanical Property Measurement
 •7.1 Introduction
 •7.2 Coupon Tests
 •7.3 Laboratory Simulation of Environmental Effects
 •7.4 Measurement of Residual Strength
 •7.5 Measurement of Interlaminar Fracture Energy
 •References
 •8. Properties of Composite Systems
 •8.1 Introduction
 •8.3 Boron Fiber Composite Systems
 •8.4 Aramid Fiber Composite Systems
 •8.6 Properties of Laminates
 •References
 •9. Joining of Composite Structures
 •9.1 Introduction
 •9.2 Comparison Between Mechanically Fastened and Adhesively Bonded Joints
 •9.3 Adhesively Bonded Joints
 •9.4 Mechanically Fastened Joints
 •References
 •10. Repair Technology
 •10.1 Introduction
 •10.2 Assessment of the Need to Repair
 •10.3 Classification of Types of Structure
 •10.4 Repair Requirements
 •10.6 Patch Repairs: General Considerations
 •10.7 Bonded Patch Repairs
 •10.9 Application Technology: In Situ Repairs
 •10.10 Bolted Repairs
 •References
 •11. Quality Assurance
 •11.1 Introduction
 •11.2 Quality Control
 •11.3 Cure Monitoring
 •References
 •12. Aircraft Applications and Design Issues
 •12.1 Overview
 •12.2 Applications of GlassFiber Composites
 •12.3 Current Applications
 •12.4 Design Considerations
 •12.7 A Value Engineering Approach to the Use of Composite Materials
 •12.8 Conclusion
 •References
 •13. Airworthiness Considerations For Airframe Structures
 •13.1 Overview
 •13.2 Certification of Airframe Structures
 •13.3 The Development of Design Allowables
 •13.4 Demonstration of Static Strength
 •13.5 Demonstration of Fatigue Strength
 •13.6 Demonstration of Damage Tolerance
 •13.7 Assessment of the Impact Damage Threat
 •References
 •14. ThreeDimensionally Reinforced Preforms and Composites
 •14.1 Introduction
 •14.2 Stitching
 •14.3 ZPinning
 •14.6 Knitting
 •14.8 Conclusion
 •References
 •15. Smart Structures
 •15.1 Introduction
 •15.2 Engineering Approaches
 •15.3 Selected Applications and Demonstrators
 •References
 •16. KnowledgeBased Engineering, ComputerAided Design, and Finite Element Analysis
 •16.2 Finite Element Modelling of Composite Structures
 •16.3 Finite Element Solution Process
 •16.4 Element Types
 •16.5 Finite Element Modelling of Composite Structures
 •16.6 Implementation
 •References
STRUCTURAL ANALYSIS 
191 
6.3Stress Concentration and Edge Effects
The strain variation through the thickness of the laminate defined by equation (6.23) is linear. Stresses vary discontinuously from ply to ply through the thickness as indicated in Figure 6.9. The determination of the stress in the kth ply requires the definition of the zposition of the ply in the laminate. Substitution into equation (6.23) defines the strains in the ply. These strains can then be substituted into equation (6.24) for the appropriate ply to define the stresses. These strains and stresses are defined in the laminate (x, y, z) coordinate system. When assessing failure in the ply, the stresses and strains are required in the material (1, 2, 3) axis system. Equation (6.5) for stress and equation (6.6) for strain can be implemented to achieve these transformations. Inverting the transformation in equation (6.5) gives the required relation:
0"2 
= 
S 2 
C 2 
  2 C S 
O'y 
'/'12 

  C S 
C S 
C 2   S 2 
'Txy 
6.3.1Stress Concentration Around Holes in Orthotropic Laminates
A common feature with isotropic materials is the stressraising effect of holes and changes in geometry that modify the load paths. Several analytical solutions for the stresses around holes in (symmetric) orthotropic laminates are cited in Ref. 7. Details of the derivations of these are given in Ref. 10. It turns out that the value of the stress concentration factor (SCF) depends markedly on the relative values of the various moduli. This can be illustrated by considering the case of a
circular hole in an infinite sheet under a uniaxial tension in 
the 
xdirection 

(Fig 
6.10). Here, the stress concentration factor at point A 
in 
Figure 6.10 
( a = 
90°), defined as the ratio of the average stress through the thickness of the 
laminate to the average applied stress grx, is given by the following formula:
SCF = K r  O'xmax_ 1 + 2 + (6.33)
~rx
The stress concentration factors for the laminates of Table 6.1 have been calculated from this formula, and the results are shown in Table 6.3.
For comparison, the SCF for an isotropic material is 3. As can be seen, when there is a high degree of anisotropy (e.g., an all 0 ° laminate), SCFs well in excess of that can be obtained. It should also be pointed out that, as the laminate pattern changes, not only does the value of the SCF change, but the point at which the SCF attains its maximum value can also change. Whereas for the first four laminates of Table 6.3, the maximum SCF does occur at point A, for the remaining laminate the maximum occurs at a point such as B in Figure 6.10.
Care should be taken when relating these results to the strength of the laminate. A laminate with all ___ 45 ° plies has the lowest SCF at 2, but may also
192 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
(~x
Fig. 6.10 Stres s concentratio n o n circula r hol e in infinite tensio n panel.
have the lowest strength due to the absence o f 0 ° plies to carry the load. The best laminate has sufficient 0 ° plies to carry the load, but also _ 45 ° plies to reduce the stress concentration factor.
6.3.2 Edge Effects
Edg e effects are caused by the requirement for strain compatibilit y between the plies in the laminate. The y lea d to interlaminar shear and throughthickness peel stresses near the free edges o f the laminate. F o r example, if a laminate consisting o f alternating 0 ° and 90 ° unidirectional plies is subject to a tensile load parallel to the 0 ° fibers, then the difference in P o i s s o n ' s ratio leads to different transverse contraction, as indicated in Figure 6.11. However, the plies in the assemble d laminate are forced to have the same transverse strain by the bonding provide d by the resin. Therefore, an interlaminar shear develops between the plies, forcing the 0 ° pl y to expan d in the transverse direction and the 90 ° ply to contract. The shear stress is confined to the edge o f the laminate becaus e once the required tension Oyis established in the 0 ° ply, for example , the compatibilit y will
Table 6.3 SCF at Circular Hole in Tension Panel (Laminate Data from Table 6.1)
Layup 

SCF 
No. 0° Plies 
No. _ 45 ° Plies 
Point A 
24 
0 
6.6 
16 
8 
4.1 
12 
12 
3.5 
8 
16 
3.0 
0 
24 
2.0 

STRUCTURAL ANALYSIS 
193 

T Y 
~ x 


Z 
v 


', 
', 
~xl 



I 

  1 . 2 . ~ . . 
2 .  . r . . . . . . 


Free edge
Interlaminar 
Peel stress 

"Czy
Fig. 6.11 Ply strain compatibility forced in a 00/90 ° laminate and interlaminar shear and peel stresses at the edge of the laminate.
be ensured across the middle of the laminate. At the free edge, however, this tension stress must drop to zero if there is no applied edge stress.
The shear stress shown in Figure 6.11 is offset from the axis of the resultant of the stress Oy, and therefore a turning moment is produced. To balance this moment, peel stresses o"z develop in the laminate having the distribution indicated
194 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
in Figure 6.11. These peel stresses can cause delamination at the edge. Similar stress distributions will be identified in Chapter 9 for bonded joints and bonded doubler plates.
Interlaminar shear stresses also occur in angle ply laminates as the individual plies distort differently under the applied loads. A more thorough treatment of edge effects is contained in Ref. 1.
6.4Failure Theories
6.4.1OverviewMatrix Cracking, First Ply Failure and Ultimate Load
The prediction of failure in laminates is complex. Failure is not only influenced by the type of loading, but also the properties of the fiber and properties of the resin, the stacking sequence of the plies, residual stresses, and environmental degradation. Failure will initiate at a local level in an individual ply or on the interface between plies but ultimate failure in multidirectional laminates may not occur until the failure has propagated to several plies.
Strains in the laminate are constant through the thickness for inplane loading of symmetric laminates, or vary linearly if the laminates are subject to outofplane curvature. However, the stresses in each ply given by equations (6.7) and (6.24) depend on the modulus of the ply and vary discontinuously through the thickness of the laminate. Failure of the laminate described by a mean stress averaged through the thickness of the laminate will therefore apply only to a particular layup. The prediction of failure in multidirectional laminates usually requires the determination of strains and stresses for each ply in the material (1, 2, 3) axes for the ply. The prediction of ultimate failure then requires following the progression of failure through the laminate. A number of different types of failure therefore need to be assessed when evaluating the strength of a laminate:
(1)matrix cracking, which may have important implications for the durability of the laminate;
(2)first ply failure, where one of the plies in the laminate exceeds its ultimate stress or strain values;
(3)ultimate failure when the laminate fails; and
(4)transverse failure or splitting between the layers of the laminate.
Matrix cracking depends on the total state of stress or strain in the matrix. It depends on the residual stress in the matrix due to the curing processes as well as stress and strain due to mechanical loads. For example, in a thermoset laminate cured at elevated temperature, the resin can be considered to cure at or near the glass transition temperature. Because the thermal expansion coefficient of the matrix is much higher than that of the fibers, cooling to room temperature introduces tension into the matrix as it tries to shrink relative to the fibers. Matrix cracking under load then usually occurs at the interface between the most highly loaded ply aligned with the load direction and an offaxis ply.
STRUCTURAL ANALYSIS 
195 
To determine the load for first ply failure, the stress and strain in the principal material (1, 2, 3) axes in each ply are determined using the theory given in Section 6.2. Hence, the problem can be reduced to establishing a criterion for the ultimate strength of a single ply with the stresses or strains referred to the material axes. As before, these stresses will be denoted by o"1, o2, and r12. A number of welltried theories, including maximum stress and maximum strain, are discussed in the subsequent sections.
It is important to note that failure of the first ply does not necessarily constitute failure of the laminate. The stiffness of the failed ply can be reduced, say, to a defined percentage of its undamaged value, and the laminate reanalyzed to check whether the remaining plies can carry the load. I f the load can be carried, the applied is increased until the next ply fails. When the load cannot be carded, ultimate failure has occurred.
The prediction of throughthickness failure has proved more difficult. This transverse failure occurs in the matrix. It is failure of the resin in either shear or tension. It depends on the total state of stress or strain in the matrix, including the stresses introduced by manufacturing of the component. Several approaches will be discussed in the following sections. When a flaw is present, a fracture mechanics approach is used to predict the growth of the flaw leading to delamination and structural failure. In the fracture mechanics approach, the strain energy release rate is determined and compared with the critical value for the matrix material. The approach has proved useful for predicting stiffener separation and delamination growth. 12
6.4.2 StressBased Failure Theory
Stressbased failure theory can be classified into two categories: maximum stress theories 1316 and quadratic stress failure theories.17'18 The stresses are first determined for each ply and transformed to the material (1, 2, 3) axes.
Maximum stress theory directly compares the maximum stress experienced by the material with its strength. The maximum stress across a number of failure modes is compared with the strength in each failure mode. First ply failure will not occur if:
//0"1 
Ioll 
02 
[o2l Is121~ 


maxL 
,l 
l, 
,l l,l l) 
1 
(6.34) 
The quadratic failure criteria include the affect of biaxial (multiaxial) load. The most used quadratic failure theories are:
TsaiHill Theory
O~1 
O102~_._~ ..[_(~'12~ 2 




X 2 
X2 
~,S~2] < 
1 
(6.35) 

If o'1 > 0, X = Xr; otherwise, 
X = 
Xc. I f o2 > 
0, Y = 
Yr', otherwise, Y = 
Yc. 

This failure criterion is a generalization of the 
von 
Mises yield criterion 
for 
196 COMPOSITEMATERIALSFORAIRCRAFTSTRUCTURES
isotropic ductile metals. When plotted with or1 and tr2 as the axes and with constant values of T12/S12 , this equation defines elliptical arcs joined at the axes.1 A more general theory can be developed based on an interactive tensor polynomial relationship. The TsaiWu criterion is invariant for transformation between coordinate systems and is capable of accounting for the difference
between tensile and compressive strengths. 1
TsaiWu Theory 17
FlO'l ÷ F2tr2 ÷ FllO'~l÷ F220~2÷ F66q2 ÷ 2F120"10"2 < 1 
(6.36) 
The TsaiWu coefficients are defined as follows:
1 1
F1 = ~TF Xc
1 1
F2 =~r + ~C
Fll  
1 

XrXc 



Fz2  
1 

YrYc 




1 

F66 '~12 
The coefficient F12 requires biaxial testing. Let Orbiaxbe the equal biaxial tensile stress (trl = tr2) at failure. If it is known, then:
El2 
~ 1 
1  
1 +~1c + ~,1~r+ ~ 7 O'biax÷ ~Xr~c+ y~yT) biax) 
otherwise, 






F12 _ ~ _ f l ~ 
where 
 1.0 < f l 
< 
1.0. The default value o f f 1 is zero. 
The maximum stress theories define simple regions in stress space. Stresses lying inside the limits defined by the solid lines in Figure 6.12 will not cause failure. Failure occurs for combinations of stresses that lie outside the failure envelope. The polynomial theories define elliptical regions. The plot appearing as a dashed line in Figure 6.12 is for the TsaiWu criterion for combinations of direct stress with zero shear stress. In this case, the ellipse crosses the axes at the four points corresponding to Xr, Xc, Yr, and Yc.
6.4.2.1 StressBased Theories: Considering Actual Failure Modes.
The TsaiHill and TsaiWu criteria do not identify which mode of failure has

STRUCTURAL ANALYSIS 
197 

02 

T s a i  W u 

Maximum 
f ' =  0 . 5 
YT 
stress 
~...... I ' ~   .
/ 
Y c 
T s a i  W u 
TI2 = 0 
f'=O 

Fig. 6.12 Stress failure envelopes 
for a typical unidirectional carbon fiber. 
(Xr = 1280 MPa, Xc = 1440 MPa, YT 
  57 MPa, Yc = 228 MPa) 
become critical. Failure theories in the second category treat the separate failure modes independently. The maximum stress criteria and the HashinRotem failure criterion treat the separate failure modes independently. 15'19
The twodimensional HashinRotem failure criterion has the following components for unidirectional material. For tensile fiber failure (O'll > 0):
//O'11x\2 
//7"12~ 2 


~Xr~) +~S~lz) 
= 1 
(6.37a) 

For compressive fiber failure (O'11 < 0): 



Xcc] = 1 

(6.37b) 

For tensile matrix failure (o'22 > 0): 



//O'22x~2 
/'r12"~ 2 
= 1 
(6.37c) 
~Yr~) + ~ 1 2 ) 

For compressive matrix failure (O'22 < 
0): 


2~) +Lt2~;~l  J ~ + t ~ } = 1 
(6.37d) 
198 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
For throughthickness failure, the combination of throughthickness stresses predicts delaminations will initiate when:
//0"33"~ 2 
//Or23~ 2 
//O"31"~ 2 
ts ) 
+tg) 
=' 
Here ~rll, tr22 and r12, are the longitudinal stress, transverse stress, and shear stress, respectively, and X, Y, Z, and S are the longitudinal strength, transverse strengths (Z is through thickness), and shear strength, respectively, that are obtained from testing. The subscripts T and C refer to tension and compression mode, respectively.
If the matrix failure parameter is satisfied first, then an initial crack forms in the matrix.
Zhang 2° separated the through thickness mode into stear and tension. For interlaminar shear failure occurs when:
~ 1 3 + ~3 > interlaminar shear strength
For interlaminar tension:
O'p~el_ 1 
(6.38) 
Zr
6.4.2.2StressBased Methods: Application to Laminates. To predict ultimate failure, the lamina failure criterion is applied to examine which ply undergoes initial failure. The stiffness of this ply is then reduced and the load is increased until the second ply fails. The process is repeated until the load cannot be increased indicating the ultimate failure load has been reached. Residual stresses can be taken into account at the laminate level.
Hashin and Rotem 15 used a different stiffness reduction method for predicting ultimate failure. A stiffness matrix represents the laminate where the stiffness of the cracked lamina decreases proportionally to the logarithmic load increase in the laminate. Residual stresses are considered, and a nonlinear analysis is used.
Liu and Tsai is use the TsaiWu 17 linear quadratic failure criterion. The failure envelope is defined by test data. The data are obtained from uniaxial and pure shear tests. After initial matrix failure, cracking in the matrix occurs. The stiffness is reduced for the failed lamina by using a matrix degradation factor that is computed from micromechanics. This process is repeated until the maximum load is reached. Thermal residual stresses, along with moisture stresses, are estimated using a linear theory of thermoelasticity. This assumes that the strains are proportional to the curing temperature.
Throughthickness failure is failure in the matrix caused by tensile stresses perpendicular to the plies. A typical example is shown in Figure 6.13. The delamination can be predicted by the interlaminar tension criterion of Zhang. 2°
STRUCTURAL ANALYSIS 
199 
d¢lamination
Fig. 6.13 Interlaminar failuresplitting in a curved beam.
Wisnom et al.21'22 use a stressbased failure criterion to predict throughthickness failure in composite structures. This matrix failure criterion uses an equivalent stress oe, calculated from the three principal stresses:
1
4 ~ 2 . 6 [(O"1   0"2)2 "~ (0"2   
0"3)2 "q (0"3   
0"1)2 "q 0.6~(0"1 + 0"2 "q 0"3)] 


(6.39) 
Interlaminar strength is considered to be related to the volume of stressed material. Therefore, the stressed volume is taken into account using a Weibull statistical strength theory. The criterion can be applied to threedimensional geometric structures with any layup. Residual stresses and the effect of hydrostatic stress are accounted for.
6.4.3StrainBased Failure Theories
The simplest strainbased failure theories compare strains in the laminate with strain limits for the material.23'24 Failure occurs if
, 
e2 
, /312 ~ = 1 
(6.40) 
m a x ( e  ~ r ' e ~ c ' ~ 
e2c 
Y12/ 

where the subscripts T and C, as before, refer to critical strains for tension and compression and T12 to critical shear strain.
The failure envelope for this failure criterion is sketched in Figure 6.14a. I f the Poisson's ratio for the laminate is nonzero, tensile strain of the laminate in the 1 direction will be accompanied by contraction in the 2direction. Transforming the failure envelope from strain axes to stress axes therefore leads to the distorted failure envelope shown in Figure 6.14b.
Puck and Schurmann 25 have developed a 
strainbased theory for fiber failure 

in tension, including deformation of fiber in 
the transverse direction. 

1 { 
1)f12 
  "~ 
+ 
= 1 



STRUCTURAL ANALYSIS 

201 

where: 









J l = 
e x 1 ~:y 1 8z 
= 
~1 F 82 t I~3 




(6.41) 

J2 = 
~x'~y qSyez Jfezl?,x ~e2y 
~e2z 
  ~ e 2 




= 
e 1 8 2 + e 2 e 3 
+ 
e 3 e l 





(6.42) 

1 

1 
2 
1 
2 
1 
2 
(6.43) 
J3 = exSyez + 3 SxySyzezx  4 exeyz  
4 
eYezx   
4 
ezexY = e l e z e 3 
6.4.3.2 First Invariant Strain Criterion for Matrix Failure. Obviously, the simplest criterion of such a kind is a function of the first invariant strain Ja, which indicates the part of the state of strain corresponding to change of volume. However, it is well known that a material would not yield under compressive hydrostatic stress; consequently, this first invariant strain criterion is applicable only to tensiontension load cases experiencing volume increases.
6.4.3.3 Second Deviatoric Strain Criterion. To consider material yielding by the part of the state of strain causing change of shape (distortion) and to exclude the part of state of strain causing change Of volume, a function of the second deviatoric invariant strain J~ has been suggested where:
1 
~:y)2 "J7 (/3y   EZZ)2 qL ( e z _ 
EZx)2 ) 

4 = 6 ( ( ~ x   

1 2 
1 2 
1 2 
(6.44) 
4 exy  
4 8yz  "4ezx 
A more convenient form for use as a failure criterion is:
~crit ~ 
V/~ 2 






~ 
3 2 
3 
2 
3 
(6.45) 
~ 
2 

( ( S x   gy) 2 ..1_ (By   gZ) 2 + 
( e z   8x ) z )   ~ 8xy  ~8yz  ~ t3ZX 
This criterion can be simplified using principal strains to:
~eqv = ~/((~31   
~32)2 "~ (~ 2   
e 3 ) 2 + ( e 3   
e l ) 2 ) / 2 
202 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
This equivalent strain, often referred to the Von Mises shear strain, is a combination of invariants:
•eqv ~" ~ 1 2  3J2
Consequently, it is also invariant to any transformation of axis.
6.4.3.4 SIFT Applied to Laminates. Use of the strain invariant failure criteria for composite laminates 3° is a break from traditional methods because it considers three planes of strain as opposed to the conventional maximum principal strain. Two mechanisms for matrix failure are considered. These are dilatational failure, characterized by the first strain invariant, J1, and distortional failure, characterized by a function of an equivalent shear strain, •eqv. Initial failure occurs when either of these parameters exceeds a critical value. The calculation of strain includes micromechanical models that take into account residual stresses and a strain amplification factor that includes strain concentration around the fiber. The criterion is a physicsbased strain approach, based on properties at the lamina level. It can be applied to threedimensional laminates with any layup, boundary, and loading conditions.
Gosse and Christensen 27 undertook several test cases on laminates, each with different layups, for verification of the strain invariant failure criterion. These tests gave a good correlation between interlaminar cracking and the first strain invariant. HartSmith and Gosse28 extended the S1FT approach to map matrix damage to predict final failure. This is done using a strainenergy approach.
6.4.4 Matrix Failure Envelopes
The matrix failure envelope27 for the SIFT criterion can be seen in Figure 6.15. When the cylindrical section is cut by the plane formed by the first two principal axes, an ellipsoid is formed. The ellipsoidal region of the envelope is governed by shear components of strain characterized by the equivalent strain,
eeqv. The 
45 ° 
cutoff plane, dominated 
by 
transverse tensile strain, 
is 
characterized by 
the first strain invariant, J1. 



The 
insert 
in Figure 6.15, developed 
by 
Sternstein and Ongchin, z9 is 
a 
failure envelope for polymers constrained within glass fibers, where the strain in the 3direction is equal to zero. When the SIFT failure envelope is transferred to stress axes both sections become segments of an ellipse as indicated in Figure 6.16.
6.4.5Comparison of Failure Prediction Models
Soden et al.31 have compared the failure predictions achieved by several theories and compared them to experimental results. 31'32'34"35 Almost all of the failure envelopes presented give an ellipsoidal shape in the negative stress region corresponding to shear loading. Transverse tensile loading causes failure in the



STRUCTURAL ANALYSIS 
203 
e2 


Cutoff governedby 




J1 invariant 




El 




~1 
Space 
I 
\~ 
I~ 
p l a n e l n t e r s e cIt 2 i t h i .~~l "~ ( 

~ 
e , = ~ = ~ 
Nofailure 


I 
i 




, 
t  ' I ~ 



predictedfor 
~ 

. .  ~ 

I 

triaxial 
~ 
 




compression 



f 
I 
% 
Seconddeviatoric
strain envelopewith
axisonspace diagonal
Fig. 6.15 The SIFT matrix failure envelope.
positive stressstrain region. 3° SIFT represents failure in this region with a cutoff plane characterized by the first strain invariant J1, whereas most of the other failure theories continue with either an eUipsoidal shape or a curved, irregular shape.
6.5 FractureMechanics
In the fracture mechanics approach, failure is predicted to occur when a crack grows spontaneously from an initial flaw.33 This approach has found application in predicting stiffener debonding 36 and for predicting interply failures.
Fracture toughness and crack growth was discussed in Chapter 2. It is apparent from that discussion that cracks are likely to grow parallel to the fibers (splitting) and parallel to the plies (delamination). Failure can also occur in assembled structures in adhesive bonds between the components. The prediction of when a delamination or disbond will grow is important for the assessment of damage tolerance where the initial defect can be assumed to arise due to manufacturing processes or due to impact or other damage mechanisms for the structure. The size of the defect is usually linked to the limits of visual inspection or the inspections that follow manufacture because known defects will be repaired.
204 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
(~2
Dilatation(Crazing)   governed by
J~ =el +E2Pe3
~von Mises ellipse
Fig. 6.16 SIFT failure envelope for polymeric materials.
The requirement is that damage that cannot be detected should not grow under operational loads.
The prediction of the growth of interlaminar splitting and disbonds in bonded joints is based on three modes of crack opening. Mode I is crack opening due to interlaminar tension, mode II due to interlaminar sliding shear, and mode I n due to interlaminar scissoring shear. The components GI, GI1, and Gill of the strain energy release rate, G, can be determined using a virtual crack closure technique in which the work done by forces to close the tip of the crack are calculated. If mode I and mode II crack opening is contributing to the growth, the delamination is predicted to grow when:
( G I ~ m [ G I I ~ n 

G~tc) +~G~/c ) = 1 
(Eq. 6.46) 
where m and n are empirically defined constants. The finite element analysis depicted in Figure 16.11 identifies the role that buckling of a panel and flanges of a stiffener can play in driving a disbond in a bonded joint.
6.6 Failure Prediction Near Stress Raisers and
Damage Tolerance
The behavior of carbon fiber laminates with epoxy resins is predominantly linearly elastic. However, some stress relief occurs near stress concentrations that is similar to the development of a plastic zone in ductile metals. Microcracking in the laminate softens the laminate in the vicinity of the notch. In the case of
STRUCTURAL ANALYSIS 
205 


(7 


t 
t 
t 

o
Fig. 6.17 Reference axes for a hole in an orthotropic panel under umform tension.
holes in composite laminates, two different approaches have been successfully developed to predict failure based on the stress distribution. These are the average stress failure criterion and the point stress failure criterion.
Consider a hole of radius R in an infinite orthotropic sheet (Fig. 6.17). If a uniform stress o is applied parallel to the yaxis at infinity, then, as shown in Ref. 21, the normal stress try along the xaxis in front of the hole can be approximated by:
(6.47)
where KTis the orthotropic stress concentration factor given by equation (6.33). The average stress failure criterion4°'41 then assumes that failure occurs when the average value of try over some fixed length ao ahead of the hole first reaches
the unnotched tensile strength of the material. That is, when:
1 [R+ao
  
try(X, O ) d x = (To 
ao JR 

206 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
Using this criterion with equation notched strength as:
crN
tro 
2   ~ 2 _ 
where:
(6.47) gives the ratio of the notched to un
2(1  ~b)
~ 4 Jr ( K T   3)(~b 6   t~8)
R
R + a o
In practice, the quantity ao is determined experimentally from strength reduction data.
The point stress criterion assumes that failure occurs when the stress oy at some fixed distance do ahead of the hole first reaches the unnotched tensile stress,
O'y(X, O)]x=R+do = O"o
It was shown in Ref. 40 that the point stress and average stress failure criteria are related, and that:
ao = 4do
The accuracy of these methods, in particular the average stress method, can be seen in Figure 6.18, where ao was taken as 3.8 mm. The solid lines represent predicted strength using the average stress criterion, and the dotted lines are the predicted strengths from the point stress method. Tests in Ref. 41 were carried out on various 16ply carbon/epoxy laminates (AS/35015) with holes. The laminates were: ( 0 / ± 4 5 2 / 0 / + 45)s, (02/_+ 45/02/90/0)s, and (0/_+ 45/90)2s. The results are shown in Table 6.4 and are compared with predicted values using the average stress method with ao 2.3 mm.
1.0 
(0 / +4 5 / 9 0 ) 2 S T 3 0 0 / 5 2 0 8 

k 

0.8 " ~ 
_ 
o 0 = 4 9 4 M P a 
O N
0 0
0.6 
Yl 
~ 





/ a°=3"$mm 








0.4 
_ 


z " " 
.to" 
" . . . . . . . . . . . . . 

0.2 
~ . % 
. 









x 







0.0 
I 
I ' ~ '  '10 
I 
I 
I 
I 
I 
I 
I 



2.5 

5.0 
7.5 

10.0 

12.5 
Hole radius, R (mm)
Fig. 6.18 Comparison of predicted and experimental failure stresses for circular holes in ( 0 / _ 45/90)2s, T300/5208.
Тут вы можете оставить комментарий к выбранному абзацу или сообщить об ошибке.
Оставленные комментарии видны всем.